ULTRASONIC PHASED ARRAY SIMULATIONS OF WELDED COMPONENTS AT NASA
D. J. Roth1, R. P. Tokars1, R. E. Martin2, R. W. Rauser,3 J.C. Aldrin4 1NASA Glenn Research Center, Cleveland, OH 44135 2Cleveland State University, Cleveland, OH 44115 3University of Toledo, Toledo, OH 2368143606 4Computational Tools, Inc., Gurnee, IL 60031
ABSTRACT. Comprehensive and accurate inspections of welded components have become of increasing importance as NASA develops new hardware such as Ares rocket segments for future exploration missions. Simulation and modeling will play an increasing role in the future for nondestructive evaluation in order to better understand the physics of the inspection process, to prove or disprove the feasibility for an inspection method or inspection scenario, for inspection optimization, for better understanding of experimental results, and for assessment of probability of detection. This study presents simulation and experimental results for an ultrasonic phased array inspection of a critical welded structure important for NASA future exploration vehicles. Keywords: nondestructive evaluation, computational simulation, ultrasonics, weld, modeling, phased array PACS: 81.70.Ex
As NASAs Constellation Program proceeds to develop new crew and launch vehicles, many inspection and nondestructive evaluation challenges will be encountered. Ultrasonic testing will play a role in the inspections of space flight hardware such as beams, welds, lugs, and other critical structures. NASA Glenn Research Center is involved in building the upper stage simulator (USS) for the Ares 1-X test rocket scheduled to launch in 2009. The upper stage is composed of multiple USS segments that will be stacked and attached to each other. The USS segments have critical welds that attach the skin half-cylinders, flange portions, and the skin to the flange. In this study, the skin-to-flange weld is of concern.
The skin-to-flange weld is required to pass a hand-held ultrasonic A-scan inspection for certification. Here, the modeling and use of phased array ultrasonics to perform such an inspection is addressed as an alternative to A-scan inspection. Phased array inspection is gaining wide acceptance and has many advantages over conventional A-scan inspection including the ability to perform scanning with no mechanical movement, the ability to perform angular (sectorial) scans and dynamic focusing, greater ability to inspect complex shapes and difficult-to-inspect areas, and two-dimensional visualization of results. Simulation and modeling will play an increasing role in the future for nondestructive evaluation in order to better understand the physics of the inspection process, to prove or disprove the feasibility for an inspection method or inspection scenario, for inspection optimization, for better understanding of experimental results, and for assessment of probability of detection. .
TEST SAMPLE A skin-to-flange test sample of pressure vessel steel variety was fabricated. The skin and flange portions were approximately 12 mm and 25 mm thick, respectively. The skin portion was double-beveled at one end, 45o each side, and butted to the thicker flange. Flux core arc welding (FCAW) was performed to attach the skin to the flange - the interior and exterior areas flanking the bevels of the skin were filled with weld metal of a similar composition to that of the base steel. The external weld was shaved to make the transition from skin to flange flat. Figure 1 shows a photograph of the interior of an Ares USS segment and a solid model of the test part. A side-drilled hole (SDH) approximately 40 mm in length and 1.61 mm in diameter was located at one end of the part, simulating lack of fusion in the weld.
___12 mm (a) (b)
FIGURE 1. (a) Actual photograph of interior of Ares USS segment and (b) solid model for the skin-to-flange test sample. PHASED ARRAY ULTRASONIC METHOD The General Electric (GE) Phasor XS portable ultrasonic flaw detector (figure 2a) was used for the actual test part inspection. Ultrasonic phased array transducers are made of multiple crystals that are electronically pulsed in a sequence using a specified delay between pulses to create linear scanning, beam steering, and / or focusing capability. Phased array probes generally consist of a transducer and wedge. The transducer employed was a 32 crystal-element linear phased array type with 5 MHz flat focus. The total aperture was 16 mm x 10 mm. The element width was approximately 0.45 mm and the gap between elements was approximately 0.05 mm. Only 16 of the 32 elements are active at any one time as 16 pulser-receivers are available in the instrument. The active aperture area was thus 8 mm x 10 mm. The transducer was attached to a wedge made of Rexolite plastic with incidence angle of approximately 36o and subsequent shear wave refraction angle into steel of approximately 54o. Note that an incidence angle of 36o results in a setup beyond the critical angle for longitudinal waves so longitudinal waves are not of concern in this study. Figure 2b shows a photograph of the probe sitting on the external skin portion of the skin-to-flange test sample. This is the single-sided inspection scenario for an actual inspection of the welds whether using A-scan or phased array methods. A sectorial scan with range 40o to 75o was performed. The probe was moved manually by hand along the exterior surface of the skin in order to determine whether an indication related to the SDH in the interior weld was observed.
(a) (b) FIGURE 2. (a) The General Electric (GE) Phasor XS portable ultrasonic flaw detector and (b) Phased array probe positioned on the external side of the skin of the skin-to-flange test part. ADDITIONAL ULTRASONIC TESTING 5 MHz shear wave ultrasonic velocity and attenuation coefficient measurements were performed on the test sample skin (base steel) and also on a flat sample of the weld steel using a precision contact ultrasonic method . The shear wave velocity values for the base steel and weld steel were measured to be 0.325 cm/sec and 0.328 cm/sec, respectively, the difference of which is close to the measurement uncertainty for the velocity measurement method. The velocity value for the base steel was used as a setup parameter in the Phasor, and the velocity values for both base and weld steels were used in the ultrasonic model as described below. ULTRASONIC MODELING
In this investigation, CIVA 9.0 software developed by the French Atomic Energy Commission (CEA) was utilized to model the phased array ultrasonic inspection. The CIVA software allows bulk wave beam field predictions using the elastodynamics pencil method and defect response predictions using Kirchhoff, GTD or Born models for beam/defect interaction [3 - 10]. The software has many powerful options available including the ability to compute delay laws for phased array ultrasonic setups [11,12] and the ability to overlay resulting beam profiles and beam/defect responses onto the model of the part. Components requiring defect response predictions need to be either imported as two-dimensional DXF files or drawn in two-dimensional profile in the computer-aided-design (CAD) facility included in the CIVA software. After the two-dimensional profile is created or imported, it is subsequently extruded to create the three-dimensional solid model. Three-dimensional solid models can be imported into CIVA, but only for beam field predictions at this time. A reasonable two-dimensional profile facsimile of the skin-to-flange test part was drawn using dimensions from the actual test part in the CIVA CAD facility (figure 3). For the CAD model, all sides were color-coded as front, back, side, and interface so that the ultrasonic probe attached itself properly, and the beam field and defect response predictions were calculated correctly. The four zones shown in the two-dimensional profile consisted of two base steel zones and two weld zones. Each was assigned the appropriate ultrasonic velocity as measured for the base and weld steels. The CIVA software has interface screens for the user to describe the transducer crystal element characteristics and geometry, phased array crystal assembly, inspection/scan parameters, wedge material and geometry, test sample material and geometry, flaw material and geometry, and computation parameters. The model parameters selected matched closely with actual experimental parameters.
The half-skip sound path interaction with the defect was chosen in the computation parameters. When the half-skip option is chosen, beam-flaw interactions that are in the direct sound path from the probe to the defect and vice-versa are considered. Additionally, waves incident on defects after reflection off the bottom surface are also taken into account. Reflections off the bottom surface from the probe towards defects are in this case considered as well as reflections off the bottom surface from the defects towards the probe. This option therefore enables the computation of corner echoes, or more generally, echoes resulting from the inward and/or outward reflection off defects via the bottom surface. Therefore, for the half-skip option, the echoes taken into account can include the specular reflections, tip diffractions, and corner-like echoes.
Back wall echoes were included in the computation (surface echoes were not included). At the 40o to 75o sector in steel, shear waves are the active wave mode as previously mentioned and were selected as the wave mode for modeling. A computation zone was selected that encompassed the weld area. Computation accounted for mode conversion, but did not account for material noise, attenuation, or shadowing